STRENGTH TESTS ON ACETYLATED ASPEN FLAKEBOARDS
STRENGTH TESTS ON ACETYLATED ASPEN
FLAKEBOARDS EXPOSED TO A
Roger M. Rowell
John A. Youngquist
Supervisory Research General Engineer
U.S. Department of Agriculture, Forest Service
Forest Products Laboratory2
Madison. WI 53705-2398
Wood Research Institute
Uji, Kyoto, Japan
(Received May 1987)
Aspen flakeboards made from control flakes and acetylated flakes at 18% acetyl weight gain using
phenol-formaldehyde or isocyanate adhesives were subjected to a bending creep test under progressive
brown-rot fungal attack with Tyromycespalustr~s.Deflection of the boards was measured as a function
of time until failure. Isocyanate-bonded control flakeboards failed in an average of 26 days, while
isocyanate-bonded acetylated boards showed little deflection after 100 days in test. Average weight
loss of isocyanate-bonded control boards at failure averaged 6.2%, while the acetylated boards showed
about 1.OO/oweight loss at the end of 100 days. Phenol-formaldehyde-bonded control flakeboards failed
in an average of 76 days, while acetylated boards showed little deflection after 100 days in test. Average
weight loss of phenol-formaldehyde-bonded control boards at failure averaged 8.6%, while the acetylated boards showed no weight loss after 100 days.
Chemical modification, acetylation, flakeboard, aspen, strength, fungi, mechanical prop-
Much of the laboratory test data published on decay of wood uses methods
based on weight loss after a certain period of time in the presence of single or
mixed organisms. It is known, however, that, for brown-rot fungal attack on solid
wood, large strength losses occur at very low wood weight loss (Cowling 1961).
A test method has been developed to determine strength losses in wood while
under attack by a brown-rot fungi (Imamura and Nishimoto 1985). The test
method determines deflection under load in a bending creep apparatus, coupled
with fungal attack. The test is run until wood failure or a maximum of 100 days.
I This article was written and prepared by U.S. Government employees on official time, and it is
therefore in the public domain and not subject to copyright.
* The Forest Products Laboratory is maintained in cooperation with the University of Wisconsin.
Woodand Ftlrcv Scicncc~.20(2). 1988. pp 266-271
B 1988 by the Soc~etyof Wood Sclence and Technolog)
Rrntc~Ilm a / .- S T R E N G T H TESTS O N ASPEN
Load and displacement gau!
\Tray for water
A testing device for bending creep measurement coupled with fungal attack. (ML86 5398)
In a recent study, flakeboards made from acetylated southern pine and aspen
flakes showed very little weight loss in both standard ASTM D 1413 soil block
tests with the brown-rot fungus Gloeophyllum trabeum and in fungal cellar tests
with brown-, white-, soft-rot fungi and tunneling bacteria (Rowel1 et al. 1987).
Since strength losses can be high even at low weight losses, it was of interest to
determine strength losses in acetylated flakeboards.
The purpose of this investigation was to apply the bending creep strength test
to aspen flakeboards made using either phenol-formaldehyde or isocyanate adhesive with control and acetylated flakes.
Reaction of flakes and board production
Oven-dry aspen flakes (all from one commercial batch) were acetylated using
the dip procedure as described earlier (Rowel1 et al. 1986). Flakes with acetyl
weight gains of 18% (based on the original oven-dry weight) were produced.
Control and acetylated flakes were made into flakeboards using the computercontrolled laboratory press as previously described (Youngquist et al. 1986). Each
board was made with a density of approximately 640 kg/m3, using either phenolformaldehyde resin (5%) or isocyanate resin (3% based on oven-dry weight of
control or acetylated flakes). The outer 3 cm were cut from each side of the
flakeboards; then three specimens (5-cm x 35-cm x 1.25-cm) for each test were
cut from the remaining board.
Bending creep test
The test boards were subjected to bending creep tests under progressive fungal
attack in a newly designed decay chamber (Imamura and Nishimoto 1985) (Fig.
1). The chamber consisted of a metal-wire frame, covered with a polyethylene
bag and a porous plug of silicon rubber. The brown-rot fungus Tyromycespalustris
(Berk. et Curt) Murr, a standard strain for Japanese Industrial Standard (JIS)
A- 9302- 1976, was used for decay attack. Mycelial fragments prepared from shake
WOOD AND FIBER SCIENCE, APRIL 1988, V . 20(2)
LOU&which caused initial deflection of 1 rnrn in bending creep tests.
Bending stress calculated from specimen dlmenslons. The load recorded after inoculation but before incubation.
culture were spread on the bottom tension surfaces of the sterilized flakeboards.
A tray filled with sterilized water was set at the bottom of the chamber to keep
the specimen in a moist condition.
Load was applied at the center of each specimen outside of the decay chamber.
The load applied to each test specimen was that amount to cause 1-mm initial
deflection. Deflection of the board at the center of the span length (300-mm) was
measured regularly with an electric dial-gauge as a criterion to determine performance. The bending creep test was carried out until the flakeboard broke under
load or 100 days, whichever came first. The test apparatus was maintained in a
conditioned room at 26 C, which was suitable for the incubation of the fungus.
After failure or 100 days, oven-dry weight loss was determined on each flakeboard.
RESULTS AND DISCUSSION
Loading stresses to cause an initial deflection of 1 mm (1/300 of the span length)
in each test specimen ranged from 22 to 44 kg/cm2 (Table 1).
Deflection-time curves for flakeboards made with isocyanate resin are shown
in Fig. 2 and with phenol-formaldehyde in Fig. 3. These curves express time as
a logarithm. There is an initial increase of deflection for both control and acetylated
flakeboards, then a stable zone, and finally, for control boards a steep slope to
The time to failure for the isocyanate-bonded control flakeboards ranged from
15 to 43 days (Table 2). Even though this range was large, the deflection-time
curves (Fig. 2) for a given set of experimental conditions are similar. After failure,
2. Period of test duration until creep fracture and weight loss of specimens.
" Not fractured for more than 100 days.
Percent weight loss after test period of 100 days.
Weight increased by less than 1%.
Percent welght loss
Rowel1 ct al. -STRENGTH T E S T S ON ASPEN
FIG. 2. Deflection-time curves of isocyanate-bonded flakeboards in bending creep tests under
A, controls; 13
0 A,acetylated. Fracture of test board is
progressive fungal attack by T. palustris.
shown by arrow. (ML86 5399)
weight loss averaged 6.2%. It can be seen in Fig. 2 that isocyanate flakeboards
made from acetylated flakes showed only a very small deflection after 100 days,
and Table 2 shows only about 1% weight loss at the end of this time.
Phenol-formaldehyde-bonded control flakeboards failed in an average of 76
days with a range of 71 to 82 days (Table 2 ) . There was much less variation in
the control test specimens as compared to isocyanate-bonded control specimens.
After failure, weight loss averaged 8.6%. Phenol-formaldehyde-bonded boards
maintained their strength longer than isocyanate-bonded boards, and all specimens failed within a short timespan of each other. Phenol-formaldehyde flakeboards made from acetylated flakes showed only a very small deflection (almost
WOOD A N D FIBER SCIENCE, APRIL 1988, V. 2012)
FIG.3. Deflection-time curves of phenol-formaldehyde-bonded flakeboards in bending creep tests
under progressive fungal attack by T. palustris.
A, controls; 0 A, acetylated. Fracture of test
board is shown by arrow. (ML86 5400)
the same as acetylated isocyanate boards) after 100 days. At the end of 100 days,
the oven-dry weight of all acetylated boards was slightly heavier (less than 1%)
than before test. This was probably due to fungal mycelia, which were not removed
Mycelium fully covered the surfaces of isocyanate control flakeboards within
1 week, but mycelial development was significantly slower in phenol-formaldehyde control flakeboards. It has been shown that unleached phenol-formaldehyde
flakeboards show some toxicity to a brown-rot fungus in soil block tests (Rowel1
et al. 1987). The presence of some soluble toxic materials in the phenol-formaldehyde-bonded flakeboards may inhibit or slow the attack by Tyromycespalustris.
This may account for the longer time to failure for phenol-formaldehyde control
flakeboards as compared to isocyanate control flakeboards.
Ro\t~lI(,I ul - S T R E N G T H TESTS O N ASPEN
Both isocyanate and phenol-formaldehyde-bonded acetylated flakeboards
showed surface mycelium colonization during the test time, but the fungus could
not attack the acetylated flakes so little strength was lost.
Since creep in wood is dependent on moisture content, it is important to determine the creep due to the moisture present in the wood separately from the
creep due to strength losses associated with decay. In developing the standard test
procedure, two sets of control specimens were used. One set had aqueous inoculum
applied to bottom tension surface of the test specimens, while a second set had
an equal amount of sterile water applied to the bottom side. The wet sterile controls
showed less than a 5-mm deflection during the 100-day test, while the controls
with decay fungus failed within the 100-day test. This showed that only a small
part of the deflection observed was associated with creep due to moisture.
Phenol-formaldehyde and isocyanate-bonded aspen flakeboards made from
acetylated flakes showed no strength or weight losses after 100 days in a decay
Aspen control flakeboards made with phenol-formaldehyde resin are more resistant to brown-rot fungus attack than are boards made with isocyanate resin.
This may be due in part to a toxic phenolic component in the phenol-formaldehyde
boards which inhibits fungal growth. Even at low weight losses (less than 10%)
both control phenol-formaldehyde and isocyanate-bonded flakeboards failed, due
to strength losses in the creep bending test, within 100 days.
These results show the importance of determining strength losses in brown-rot
fungal tests rather than weight losses. Significant strength loss occurs even at very
low weight loss. Future research will be aimed at determining the mechanism of
biological resistance due to acetylation.
E. B. 196 1. Comparative biochemistry of the decay of sweetgum sapwood by white-rot
and brown-rot fungi. USDA Forest Serv. Tech. Bull. No. 1258, p. 50.
Y., AND K. NISHIMOTO.1985. Bending creep test of wood-based materials under fungal
attack. J. Soc. Materials Sci. 34(383):985-989, Japan.
R. M., G. R. ESENTHER,
D. D. NICHOLAS,
AND T. NILSSON. 1987. Biological resistance of
southern pine and aspen flakeboards made from acetylated flakes. J. Wood Chem. Technol. 7(3):
AND R. SIMONSON.1986. A simplified procedure for the acetylation of
hardwood and softwood flakes for flakeboard production. J. Wood Chem. Technol. 6(3):427448.
J. A., A. KRZYSKIK,
AND R. M. ROWELL.1986. Mechanical properties and dimensional
stability of acetylated aspen flakeboard. Holz Roh Werkst. 44(12):453-457.